CHALLENGES OF HOMOGENEOUS ELECTROCATALYSTS FOR HYDROGEN EVOLUTION – EVALUATION AND APPLICATION FOR USE IN EARTH-ABUNDANT
Daniel James Martin
Submitted to the Department of Chemistry as supplement to the requirements for the degree of
Bachelor of Science in Chemistry at
THE UNIVERSITY OF NORTH CAROLINA AT CHAPEL HILL May 2015
© Daniel James Martin. All rights reserved.
Foremost, to Jillian Dempsey: had you asked me four years ago who I wanted to be and what I wanted to do with my life, you would have found a different person. I cannot express how grateful I am to have been a part of your lab. I have learned so much, both in terms of research and personal development.
There’s been more than one occasion where I’ve shared this story, but when I chose to come to Chapel Hill, I didn’t realize how fortunate I was. I went through the motions of
classwork and homework without garnering interest or finding value in the things that I studied. It was then that I joined your group. All of a sudden my coursework became fascinating, particularly subjects that tied themselves to research. Application took hold in place of
memorization, and I saw value in what your group was trying to achieve. Their goals became my own, and it gave me a direction to strive towards.
Thank you Jill, for everything you’ve done.
To Brian McCarthy, my graduate student research advisor and my friend: you have been such a wonderful inspiration and guide. You said that I made your job easy, but really the other way around is far more true. Of all the teachers I’ve had these past few years, you have
undoubtedly been the best. You are steadfast and surefooted, and I have no doubt that you will do great things with your future. Know that you have inspired nothing less in me. I hope your next undergraduate realizes just how lucky he or she is to have you.
me and the other undergraduates. I wish you both the best of luck next year and looking forward to seeing what comes your way.
To Kelly, Chris, Yejee, Ana, and Dan: thank you all for your guidance, laughs, and cheerful spirits. Against the odds and ends and frustrations of research, never let them falter.
To Dr. Carolyn Morse and Dr. Domenic Tiani: thank you both for your support and encouragement these past four years. You both have driven me towards the right direction since day one, and I cannot thank you enough for your kindness.
To my family: I owe you everything. Your support, kindness, and unconditional love have provided me with the nurturing atmosphere that I needed to develop into the adult I am today. Amongst the thousands of other lessons I have learned from you, I strive to lead kindly, to care passionately, and to dream without bounds. Don’t ever stop giving me advice, or John for that matter. I am fortunate beyond words to have been a part of our family.
Acknowledgments………...III Abstract………...V Table of Contents………...VI List of Figures……….VIII List of Tables………...IX
Chapter 1. Electrochemical Reduction of Brᴓnsted Acids by Glassy Carbon in Acetonitrile…..1
Acid Reduction Measurements………....5
Reduction Potentials………7 Discussion………..10 Homoconjugation………...10 Electrode/Solvent Fouling……….12 Reduction Potentials………..13 Conclusions………18 References………..…19
Chapter 2. Electrochemical Hydrogenation of a Ni(II) Complex to Form a Surface-Adsorbed Hydrogen-Evolving Species………21
Results and Discussion………..23
Chapter 3. Synthesis and Electrochemical Characterization of Fe(N-N-SCH3)2(ClO4)2 Analogues………....43
Results and Discussion………..45
Weak-Regime Proton Sources……….50
Results and Discussion………..52
A New Oxidation……….57
References………..59 Appendix A………..A-1 Chapter 1. Experimental Details……….A-1 General Considerations………A-2 Synthesis………..A-2 Electrochemical Methods………A-4 Spectrophotometric Titrations……….A-5 References………A-5 Appendix B………..B-1
Chapter 2. Experimental Details………..B-1 General Considerations………B-2 Electrochemical Methods……….B-3 Surface Analysis Sample Preparation………..B-3 Synthesis and Characterization of 1 ………B-4
LIST OF FIGURES
Figure 1.1 Simulated cyclic voltammograms of an EC’ catalytic process………..2
Figure 1.2 Cyclic voltammograms of three acids in acetonitrile……….5
Figure 1.3 Cyclic voltammograms of 4-cyanoanilinium prewave………..6
Figure 1.4 Cyclic voltammograms of 4-chloroanilinium variability………...7
Figure 1.5 Assigning Einf by the derivative of the forward trace……….8
Figure 1.6 Cyclic voltammograms of pyridinium chloride electrode fouling………...13
Figure 1.7 Einf versus respective pKa and EHA0 values…..……….………....15
Figure 1.8 Assigning a color scale to normalized voltammogram currents………..16
Figure 1.9 Acid potential windows in acetonitrile……….17
Figure 2.1 Ni(N-N-SCH3)22+ analogues, 1 and 2………...23
Figure 2.2 Scan rate dependence of 1 without acid………...24
Figure 2.3 Free ligand reduction versus coordinated ligand reduction………..24
Figure 2.4 Cyclic voltammogram responses of 1 and prewave to CF3COOH titrations………...25
Figure 2.5 Prewave versus free ligand hydrogenation cyclic voltammetry………...26
Figure 2.6 Redox couples of 1 and 2 without acid………27
Figure 2.7 CF3COOH titrations into solutions of 1 and 2……….28
Figure 2.8 Excess CF3COOH titrations into solution of 1……….28
Figure 2.9 Rinse test for 1………..29
Figure 2.10 Conditional electrodeposition of 1……….30
Figure 2.11 Excess CF3COOH titrations using electrode treated with 1………...31
Figure 2.12 Rinse test for 2………....32
Figure 2.13 Chronoamperometry of 1 under pseudo-steady state conditions………...33
Figure 2.14 Scanning electron microscopy and transition electron microscopy of 1…………...35
Figure 2.15 Scanning electron microscopy and transition electron microscopy of 2………35
Figure 2.18 Effects of stripping wave on catalytic activity of electrode treated with 1………....38
Figure 2.19 Cyclic voltammograms of CF3COOH titrations into solutions of 1, 2, and Ni(ClO4)2………...39
Figure 3.1 Fe(N-N-SCH3)22+, 3………..45
Figure 3.2 Cyclic voltammetry of 3 without acid………..46
Figure 3.3 Fast scan rate cyclic voltammetry of 3 without acid………46
Figure 3.4 Cyclic voltammogram responses of 3 and prewave to CF3COOH titrations………...47
Figure 3.5 Rinse test for 3………..48
Figure 4.1 CF3COOH titrations into solution of 4 and peak height analysis……….…...53
Figure 4.2 Peak height rates and cyclic voltammograms versus acid pKa for use with 4……....55
Figure 4.3 Scan rate analysis of 4 and submolar CF3COOH……….……57
Figure 4.4 Acid identity dependence of oxidation peak positions……….58
Figure 4.5 Effect of 4-chloroanilinium and conjugate base titrations on oxidation peak positions……….58
Figure B.1 1H NMR of 2-Pyridyl-N-(2’-thiolophenyl)methylenimine………B-5 Figure B.2 1H NMR of 2-Pyridyl-N-(2’-methylthiophenyl)methylenimine………B-6 Figure B.3 1H NMR of 2-Pyridyl-N-(2’-methylthiophenyl)methylamine………...B-7 Figure B.4 Three-compartment bulk electrolysis cell for hydrogen detection………….……...B-9 LIST OF TABLES Table 1.1 Average acid reduction potentials vs. Fc/Fc+………..…9
Table 2.1 Prewave and direct ligand integration values for 1………26
Table 2.2 Xray-photoelectron spectroscopy elemental analysis summary………36
ELECTROCHEMICAL REDUCTION OF BR
ᴓNSTED ACIDS BY GLASSY CARBON IN ACETONITRILE
Portions of this work are excerpted with permission from:
McCarthy, B. D., Martin, D. J., Rountree, E. S., Ullman, A. C., Dempsey, J. L. Inorg. Chem.
2014, 53, 8350-8361.
Homogeneous hydrogen evolution catalysts are often evaluated electrochemically in acetonitrile, where an electrode supplies electrons and a Brønsted acid provides protons.
catalyst + 2e−+ 2HA → catalyst + 2A−+ H
A possibly serious complication in these studies is direct acid reduction by the electrode at potentials that overlap with molecular catalysis (Figure 1.1).
2HA + 2e− → H
2 + 2A− (2)
Figure 1.1 Simulated cyclic voltammograms of an EC′ catalytic process in which direct substrate reduction (acid reduction) occurs at potentials a) far from catalysis, b) slightly overlapping with catalysis, c) strongly overlapping with catalysis, and d) nearly completely overlapping with catalysis. Solid gray line indicates that only acid is present while the dotted blue line indicates that catalyst and acid are present. Simulated using DigiElch electrochemical simulation software (Gamry Instruments); α = 0.5, ks = 10,000 cm/s, kcatalysis = 10,000 M-1 s-1, [catalyst] = 0.01 M,
[substrate]0 = 5 M.
(CVs) that mimic prototypical catalytic responses,3 especially that of catalysis exhibiting substrate depletion,4 making it unclear whether the catalyst is responsible for the current enhancement. As many hydrogen evolution catalysts operate at fairly cathodic potentials, the possibility of direct acid reduction by both relatively strong and relatively weak acids becomes an even greater concern.
These issues are minimized when acid-only controls are run. Surprisingly, acid-only cyclic voltammograms are not always reported with catalytic data. The widespread use of glassy carbon working electrodes for non-aqueous hydrogen evolving catalysts may provide one reason. Glassy carbon is often cited as non-catalytic,5–7 incorrectly implying that the direct reduction of protons to form hydrogen occurs at such negative potentials as to be inconsequential. While glassy carbon indeed reduces acids at more negative potentials than platinum,8 reduction processes can still occur. Moreover, when stronger acids are employed, reduction is expected to occur at relatively positive potentials.1 While aqueous proton reduction has been extensively studied on many electrode materials, especially platinum,9,10 and remains the subject of active research,10 little data is available on the reduction of acids in acetonitrile by glassy carbon. One report described the use of different electrodes to achieve wider potential windows for acids in acetonitrile, but only data for acetic acid was shown.8
Motivated by our interest in molecular electrocatalysts for hydrogen evolution, we were interested in better understanding the potential window limits of GC. Accordingly, the goal of this work is to establish useful approximate working ranges for common acids in acetonitrile for the specific purpose of catalytic hydrogen evolution. Reduction potentials of 20 acids in acetonitrile on glassy carbon are reported along with details on the influence of water.
Results and Discussion
Two non-aqueous reference electrodes were tested: 1) a reference electrode in which a silver wire was immersed in an acetonitrile solution containing 100 mM [Bu4N][PF6] and 10 mM
AgNO3; and 2) a pseudo-reference in which a silver wire was immersed in an acetonitrile
solution containing 100 mM [Bu4N][PF6]. In both cases the silver wire and electrolyte solution
occasionally contaminate the bulk solution with silver ions, as suggested by an oxidation at approximately –0.24 V vs. Fc/Fc+. By comparison to pure silver nitrate, the contamination proved to be the stripping of reduced silver off the glassy carbon electrode. This contamination of the bulk solution with silver ions was observed to result in variable reduction potentials for some acids. Silver is likely a better catalyst for hydrogen evolution than glassy carbon; as such, any silver contamination may shift the acid reduction potential more positive.
A Ag/AgCl pseudoreference immersed in an acetonitrile electrolyte solution in a glass tube equipped with a porous Vycor frit was not used because silver chloride is somewhat soluble in acetonitrile (especially if solution chloride anions are present),11 and we wished to avoid the possibility of solution contamination by silver ions. Consequently, pseudo-reference electrode 2 was chosen for acid reduction measurements. Over a thirty minute period the pseudo-reference electrode was observed to drift 15 ± 14 mV by monitoring the E1/2 position of the
ferrocene/ferrocenium couple (0.8 to 1.8 mM ferrocene) in a 100 mM [Bu4N][PF6] acetonitrile
solution. While extensive studies were not done, the solute may influence drift rate. Electrode Fouling
Figure 1.2 Cyclic voltammograms of three acids in acetonitrile using a glassy carbon electrode showing the response of the electrode on subsequent scans. Scan rate = 100 mV/s, 100 mM [Bu4N][PF6].
Acid Reduction Measurements
To avoid electrode fouling, freshly polished and electrochemically pretreated glassy carbon electrodes were used for each CV. In a typical experiment, a number of glassy carbon electrodes were polished in alumina/water slurries, ultrasonicated, and rinsed with acetone before being brought into a nitrogen filled glovebox. Prior to adding acid, each glassy carbon electrode was electrochemically pretreated (by cyclically scanning between approximately 0.7 and –2.8 V at 100 mV/s three times in 100 mM [Bu4N][PF6] solution), and a background scan recorded in
the 100 mM [Bu4N][PF6] acetonitrile solution.
It was checked if the glassy carbon electrode surface changed over time after pretreatment. After pretreatment, a background scan was taken and the electrode was rinsed in acetonitrile. It was then left under nitrogen for two hours before the acquisition of a second background scan. Little difference was observed between the two scans.
Twenty acids over an approximately 26 pKa unit range plus water were selected for
mV/s scan rate. While detailed electrochemical measurements of these acids was not the goal of this work, below are general observations.
For two acids – benzoic acid and 4-nitroanilinium – the return sweep cathodically crossed the forward sweep. For benzoic acid this curve crossing was more pronounced at higher concentrations and less distinct at faster scan rates. 4-nitroanilinium also displayed curve crossing; however, at higher scan rates the crossing did not appear to decrease.
Anilinium, benzoic acid, 4-methoxyanilinium, and 4-cyanoanilinium reproducibly showed cathodic current peaks preceding the main reduction. Figure 1.3 shows the current response of 4-cyanoanilinium at 100 and 1000 mV/s – at 1000 mV/s the prewave increased proportionally more relative to the main reduction. Upon repeating the 100 mV/s scan, without polishing, the prewave vanished. No prewave is seen in a literature example for a solution of 10 mM 4-cyanoanilinium,12 suggesting the presence of prewaves may highly depend on small variations of the glassy carbon electrode surface. However, a concentration dependence study of 4-cyanoanilinium revealed a lack of a prewave at 5 and 10 mM but an appearance of the prewave at 25 mM.
Figure 1.3 Cyclic voltammograms of 25 mM 4-cyanoanilinium (100 mM [Bu4N][PF6]
acetonitrile solution) at 100 and 1000 mV/s showing the presence of a prewave on the forward sweep.
bromoanilinium, chloroanilinium, tertbutylanilinium, anilinium, N,N-dimethylanilinium, 4-methoxyanilinium, and p-toluenesulfonic acid monohydrate – showed substantially dissimilar CVs taken immediately after one another using only freshly prepared glassy carbon electrodes. Figure 1.4 shows one representative example for 4-chloroanilinium where the wave shape and wave position changed dramatically. To check whether or not this acid was particularly sensitive to changing electrode surfaces, both electrodes were removed, repolished and re-pretreated. Following acquisitions of two new scans in the same solution, also shown in Figure 1.4, revealed that while neither scan resembled the prior scans in location or peak current, both traced each other very closely. Repeating this measurement yielded highly variable wave shapes and positions but did not confirm that the final scans taken after a later time overlaid as shown in Figure 1.4.
Figure 1.4 Cyclic voltammograms (100 mV/s) of 25 mM 4-chloroanilinium in a 100 mM [Bu4N][PF6] acetonitrile solution using two different glassy carbon working electrodes (w.e. 1
and w.e. 2). Scan number indicates the total number of scans taken total. Reduction Potentials
Figure 1.5. Cyclic voltammogram of 25 mM acetic acid at 100 mV/s in 100 mM [Bu4N][PF6]
acetonitrile solution and the first derivative of the forward trace. The dashed vertical line denotes the inflection point potential.
Table 1.1 summarizes the inflection reduction potential Einf. for each acid studied as the
average of three independent scans measured at 100 mV/s. Values of Einf. for the various acids
Table 1.1 Average acid reduction potentials vs. Fc/Fc+ in 0.1 M [Bu4N][PF6] CH3CN on GC at 25 mM and 100
mV/s. CVs were ohmic drop corrected prior to Einf.
Acid Einf. (V)a notesb
Water not obs.
Phenol -2.60 ± 0.06
Acetic -2.36 ± 0.05
triethylammonium -2.29 ± 0.02
Benzoic -2.25 ± 0.02 c.c.; pw.
4-cyanoanilinium -2.06 ± 0.02
dimethylformamidium -2.00 ± 0.34 var.
4-methoxyanilinium -1.95 ± 0.08 pw.; var.
Salicylic -1.94 ± 0.06
N,N-dimethylanilinium -1.90 ± 0.06 var.
4-chloroanilinium -1.86 ± 0.11 var.
Anilinium -1.83 ± 0.07 pw.; var.
4-bromoanilinium -1.83 ± 0.06 var.
4-tert-butylanilinium -1.83 ± 0.05 var.
Trifluoroacetic -1.81 ± 0.03
Pyridinium -1.77 ± 0.09
p-toluenesulfonic -1.76 ± 0.15 var.
Trichloroacetic -1.56 ± 0.02
2-nitrophenol -1.24 ± 0.02 c.c.
Trifluoromethanesulfonic -1.06 ± 0.02
4-nitroanilinium -0.65 ± 0.02 c.c.
aProvided value given as the average of three
independent measurements, except for dimethylformamidium, for which eight measurements are averaged. Error given as ± one standard deviation. A minimum standard deviation of 0.02 V is given based on the observed drift of the pseudoreference in a half hour period. bAcids displaying curve crossing on the return scan are denoted c.c., pw. designates acids showing cathodic prewaves, and var. indicates acids which showed significantly different CVs in the same solution with two different glassy carbon electrodes.
Since the surface chemistry, and hence electrochemical response, of glassy carbon is complex,13 it was checked whether electrodes from an another supplier could yield different Einf.
values. Consequently, in addition to the Einf. value reported in Table 1.1 for benzoic acid found
from two other suppliers (eDAQ, 1 mm diameter GC electrode and BASI, 3 mm diameter GC electrode) using identical procedures. The eDAQ electrodes yielded an Einf. of –2.27 ± 0.02 V
and the BASi electrode gave an Einf. of –2.27 ± 0.02 V, which is similar to the –2.25 ± 0.02 V
value determined using the CHI electrodes. This suggests that small variations between different glassy carbon electrodes can result in slightly different values, however, the values reported here should still serve as useful approximate values.
Due to the weak cation and even weaker anion solvating ability of acetonitrile, dissociated species can gain additional stability by forming homoconjugated complexes with the parent compound.14,15 In the prototypical example, acid HA dissociates in solvent S to form solvated H+ (by solvent or HA) and A-, followed by association of A- with HA to form the hydrogen-bonded homoconjugation complex [A ⋯ HA]−.
HA + S ⇌ H+S + A− or 2HA ⇌ H
2A++ A− (3)
A−+ HA ⇌ [A ⋯ HA]− (4)
Homoconjugation can consequently increase the apparent acidity of the parent acid by displacing the equilibrium towards deprotonation at the expense of reducing the overall concentration of free HA.
As homoconjugation can complicate electrochemical studies of hydrogen evolving catalysts and result in multiple catalytic cyclic voltammetric waves,16 it is desirable to know at which concentrations homoconjugation is less influential. It is not feasible to generally comment at which concentrations homoconjugation becomes less appreciable for all acids, but a value of 0.001 N (0.001 M effective acidic proton concentration) was proposed.17 A parameter κ was recently suggested to provide a more specific estimate for the extent of homoconjugation:16
𝜅 = 𝐾fC0 (5)
where C0 is the total acid concentration and Kf is the formation constant of the homoconjugation
𝐾f=[[A ⋯ HA]−]
For κ ›› 1, the acid completely homoconjugates; for κ ‹‹ 1, the acid does not appreciably homoconjugate. For example, an acid with log(Kf) = 2.0 (Kf = 100) has a κ equal to 10 when
[acid]total = 0.1 M. As most catalytic studies use acid concentrations between 0.01 and 1 M,
homoconjugation is almost certainly always occurring in measurements that utilize homoconjugating acids.
Homoconjugation is expected to influence acid electroreduction. If the acid is reduced to hydrogen, an equivalent of the conjugate base is formed and the concentration of conjugate base will rapidly increase near the electrode surface, engaging in homoconjugation reactions with the parent acid if favorable and so perturbing the Kf equilibrium. These homoconjugates
([A ⋯ HA]−) may have reduction potentials different than the parent acid; along those lines of
logic homoconjugation has been suggested to produce multiple catalytic reduction waves for hydrogen evolving catalysts.16 Artero and co-workers have suggested that complications arising from homoconjugation can be successfully accounted for theoretically on an acid-by-acid basis.16
Preferably, acids should be chosen with small, or preferably nonexistent, homoconjugation properties. For example, 2-nitrophenol has very weak (or nonexistent) homoconjugation tendencies because the ortho-positioned nitro group stabilizes the neutral, undissociated phenol proton by intramolecular hydrogen bonding preferentially over hydrogen bonding with dissociated 2-nitrophenoxide.18,19 However, as detailed below, 2-nitrophenol is unsuitable for hydrogen evolution catalysis because of its very positive reduction potential. Cationic acids, which form neutral conjugate bases, may also be expected to form homoconjugated complexes more weakly, as cationic and especially neutral species are generally more easily solvated by acetonitrile than anionic species.
during catalysis will not meaningful change the concentration of A– already present. Hence, the extent of homoconjugation will be approximately the same throughout the measurement, rather than increasing in importance in the case where no conjugate base is initially present.
If acids that do not homoconjugate appreciably must be used, then using 50/50 mixtures of acid/conjugate base to reduce changes on the experimental timescale and/or using the theoretical methods developed by Artero et al. to correctly account for homoconjugation should be used.16
Electrode and Solvent Fouling
Figure 1.6 Cyclic voltammograms of 25 mM pyridinium chloride in 100 mM [Bu4N][PF6]
acetonitrile solution at 100 mV/s showing reproducibility if only freshly polished working electrodes are used. Here, two working electrodes, w.e. 1 and w.e. 2, were used.
Apart from electrode fouling, the bulk solvent composition itself can change. While little information is available on the interactions of common acids with acetonitrile, trifluoromethanesulfonic acid reacts with acetonitrile, forming a multitude of products.25 At higher ratios of trifluoromethanesulfonic acid to acetonitrile (14:1 and 2:1), over ten species were formed. At lower ratios (1:200), only acetamide was seen. It should be noted that for the 1:200 experiment the mixture of acetonitrile and trifluoromethanesulfonic acid were boiled in CD2Cl2
prior to spectral acquisition. We independently confirmed that trifluoromethanesulfonic acid reacts with acetonitrile at room temperature by 1H NMR.
These unknown degradation products could interact with a catalyst in unanticipated ways – including degrading the catalyst. It is crucial that acids be checked for possible direct interactions with the solvent and catalyst prior to reduction. Of the acids studied here, only trifluoromethanesulfonic acid is known to interact with acetonitrile and it is anticipated that the weaker acids, incapable of protonating acetonitrile, will be relatively unreactive.
The reduction potentials of 20 acids at 25 mM and 100 mV/s in 0.1 M [Bu4N][PF6]
on platinum electrodes.10,26 It should be noted that the reported values may show a small dependence on electrolyte identity; fortunately most acetonitrile electrochemistry is carried out with 0.1 M [Bu4N][PF6].
Due to the lack of reversibility, no thermodynamically precise reduction values could be assigned.27 However, it was still desirable to report reduction potential for the acids studied for comparative purposes. Reduction values were obtained by finding the maximum of the derivative of the forward scan – the inflection point, Einf.. A similar method was proposed as a
way to estimate the mid-wave potential for catalytic CVs,16 although it should be noted that the theory used in that work is not translatable to the strictly irreversible processes seen here. Alternative methods were considered, including a) taking the potential at maximum peak current, b) the potential at half peak current, and c) defining a threshold current density as the ‘onset’ potential. Peaks were not always observed, especially at higher scan rates where depletion of the acid did not occur quickly enough to result in a peak in the potential window studied. The loss of peak shape at higher scan rates is clearly illustrated for acetic acid which was measured up to 9000 mV/s. Methods a and b were consequently not chosen, and method c, setting a threshold current density, is inherently arbitrary.16 The Einf. method was chosen here for practicality. It
should also be noted that while taking the derivative of a reversible cyclic voltammogram is equivalent to a differential pulse voltammogram of the same system, this is not the case for an irreversible process. For an irreversible process equilibrium is not maintained during the forward/backward potential steps of differential pulse voltammetry, resulting in a different current response.
Using pKa values either taken from the literature or determined in the present study, Einf.
values for each acid were plotted against the appropriate pKa (Figure 1.7). Figure 1.7 also
includes a gray region which indicates where it is thermodynamically impossible to reduce an acid to hydrogen and its conjugate base. This boundary of this zone was calculated using equation 7:8
𝐸HA0 = 𝐸𝐻+/𝐻 2
0 − (2.303𝑅𝑇/𝐹) ∙ p𝐾
Where –0.028 V (vs. Fc/Fc+) was used as the value of 𝐸𝐻+/𝐻 2
.16 See reference 16 for a recent discussion of 𝐸𝐻+/𝐻
Figure 1.7 Plot of Einf. values versus the respective pKa for each acid studied. The gray region is
an estimation of the zone in which the applied potential is thermodynamically insufficient to reduce acids to hydrogen (2HA + 2e− ⇌ H
2+ 2A−). See text for details.
A linear trend is observed between Einf. values for each acid and the respective pKa
(Figure 1.7), with weaker acids having more negative Einf. values. This is consistent with linear
trends seen in DMSO6,28 and with gas phase measurements,29 supporting the thermodynamic suggestion that weaker acids require more driving force to yield hydrogen (see discussion above). 4-nitroanilinium lies relatively close to the thermodynamic boundary as compared to the main group of acids, and 2-nitrophenol occurs within the zone where hydrogen evolution should be thermodynamically prohibited. Deviation from the linearity of reduction potential versus pKa
has been observed for nitro- and cyano-substituted methylanthracenes, derivatives in which the possibility of resonance interactions between the nitro/cyano group and the aromatic system were cited as possible explanation.28 Similar resonance interactions likely apply here, possibly encouraging direct reduction to radical species which would have different thermodynamic requirements. Alternative reduction pathways involving formation of radical species are suggested to account for the deviation from linearity of some of the anilinium compounds (see discussion above).
The potential at which it is thermodynamically possible to reduce an acidic proton with known pKa was estimated using equation 7 with –0.028 V as the value for 𝐸𝐻0+/𝐻2.16 The
concentrations usually employed. Consequently, the thermodynamic region depicted in Figure 1.7 is oversimplified, as these values should be acid and concentration dependent. The thermodynamics of acid reduction to hydrogen continues to be discussed16,20,30 and further comment here is not the intended goal of this work.
The Einf. values in Table 1.1 do not accurately convey the amount of background current
passed at potentials prior to Einf., especially for acids which exhibited prewaves (Figure 1.3, see
Table 1.1). Prewaves can be explained by adsorption of the reduced product where the adsorption free energy reduces the energy – and so applied potential – needed for reduction.31 To more accurately capture the presence of background current like prewaves, an alternative method of presenting the background current passed between the minimum thermodynamic potential 𝐸𝐻𝐴0
and Einf. is shown in Figure 1.8. Here, the current has been background subtracted and
normalized relative to the current passed at Einf.. A color gradient was subsequently mapped onto
the normalized current versus potential values.
Figure 1.8 Background subtracted cyclic voltammogram of 25 mM 4-cyanoanilinium at 100 mV/s, normalized to the current measured at Einf.. The color scale was mapped onto the
normalized current values, where white indicates no current being passed above the background current and dark blue indicates the level of current passed at the inflection point.
The color scale in Figure 1.8 of 4-cyanoanilinium reflects what the Einf. value does not:
gradient color scale was generated for each acid studied (Figure 1.9) and acids were categorized into three categories: a) eight recommended acids that showed reproducible backgrounds, b) eight acids with erratic backgrounds, and c) four acids we suggest as unsuitable for electrochemical hydrogen evolution studies in acetonitrile.
Figure 1.9 Acid potential windows in acetonitrile (25 mM acid, 100 mV/s) showing the range between an approximate thermodynamic potential 𝐸𝐻𝐴0 (where proton reduction to hydrogen is thermodynamically possible) and the direct reduction potential Einf.. The color scale was
constructed by choosing a representative CV with an Einf. close to the average Einf. value and
normalizing between 0 (background current without acid, white) and 1 (current at Einf., dark
blue). Data more positive than the thermodynamic reduction potential 𝐸𝐻𝐴0 (based on equation 7)
was then removed. Prewaves and significant current prior to Einf. are visible for some acids.
Unsuitable acids: 1) The Einf. value of 2-nitrophenol was more positive than the 𝐸𝐻𝐴0 for
Figure 1.9 captures the presence of prewaves or other significant non-background current being passed prior to the Einf. value, and so highlights the fact that certain acids (e.g.,
p-toluenesulfonic acid) pass some current above background over most of the potential range while other acids (e.g., pyridinium) pass relatively little current prior to the main reduction wave. It is hoped that Figure 11 can be used to rapidly choose candidate acids such that a) the acid can be thermodynamically reduced to hydrogen at the relevant redox potential of a given catalyst and b) that direct electrode acid reduction is avoided.
The electroreduction of 20 acids plus water on glassy carbon in acetonitrile was investigated. Figure 1.9 presents the approximate potential windows in which acids may be used for catalytic hydrogen evolution while a) avoiding direct reduction and b) allowing for the thermodynamic possibility of reduction to hydrogen. Figure 1.9 additionally includes our recommendations for which acids to use, which acids give problematic backgrounds, and which acids are generally unsuitable for hydrogen evolution catalysis in acetonitrile. We reiterate that accurately determining the thermodynamic potential is more complex16,20,30 than what was considered here.
(1) Felton, G. a. N.; Mebi, C. a.; Petro, B. J.; Vannucci, A. K.; Evans, D. H.; Glass, R. S.; Lichtenberger, D. L. J. Organomet. Chem. 2009, 694, 2681.
(2) Savéant, J.-M. Elements of Molecular and Biomolecular Electrochemistry; John Wiley & Sons, Inc.: Hoboken, 2006.
(3) Savéant, J.-M. Chem. Rev. 2008, 108, 2348.
(4) Savéant, J.-M.; Su, K. B. J. Electroanal. Chem. 1984, 171, 341. (5) Treimer, S. E.; Evans, D. H. J. Electroanal. Chem. 1998, 449, 39. (6) Treimer, S. E.; Evans, D. H. J. Electroanal. Chem. 1998, 455, 19.
(7) Lessene, G.; Bordeau, M.; Biran, C.; de Montauzon, D.; Gerval, J. J. Electroanal. Chem.
2000, 490, 79.
(8) Felton, G. A. N.; Glass, R. S.; Lichtenberger, D. L.; Evans, D. H. Inorg. Chem. 2006, 45, 9181.
(9) Compton, R. G.; Banks, C. E. Understanding Voltammetry; 2nd ed.; Imperial College Press: London, 2011.
(10) Costentin, C.; Canales, J. C.; Haddou, B.; Savéant, J.-M. J. Am. Chem. Soc. 2013, 135, 17671.
(11) Coetzee, J. F.; Padmanabhan, G. R. J. Phys. Chem. 1962, 66, 1708. (12) Baffert, C.; Artero, V.; Fontecave, M. Inorg. Chem. 2007, 46, 1817.
(13) McCreery, R. L. In Interfacial Electrochemistry : Theory, Experiment, and Applications; Wieckowski, A., Ed.; Dekker, N.Y.: New York, 2013; pp. 631–647.
(14) French, C. M.; Roe, I. G. Trans. Faraday Soc. 1953, 49, 314.
(15) Coetzee, J. F. In Progress in Physical Organic Chemistry, Volume 4; Streitwieser Jr., A.; Taft, R. W., Eds.; John Wiley & Sons, Inc.: Hoboken, 1967; pp. 45–92.
(16) Fourmond, V.; Jacques, P.-A.; Fontecave, M.; Artero, V. Inorg. Chem. 2010, 49, 10338. (17) Kolthoff, I. M.; Chantooni, M. K.; Bhowmik, S. Anal. Chem. 1967, 39, 1627.
(19) Kütt, A.; Leito, I.; Kaljurand, I.; Sooväli, L.; Vlasov, V. M.; Yagupolskii, L. M.; Koppel, I. A. J. Org. Chem. 2006, 71, 2829.
(20) Appel, A. M.; Helm, M. L. ACS Catal. 2014, 4, 630. (21) McCreery, R. L. Chem. Rev. 2008, 108, 2646.
(22) Wong, R. P.; Wong, J. E.; Birss, V. I. Can. J. Chem. 2004, 82, 1536.
(23) Birss, V.; Dang, K.; Wong, J. E.; Wong, R. P. . J. Electroanal. Chem. 2003, 550-551, 67. (24) Anxolabéhère-Mallart, E.; Costentin, C.; Fournier, M.; Nowak, S.; Robert, M.; Savéant,
J.-M. J. Am. Chem. Soc. 2012, 134, 6104.
(25) Salnikov, G. E.; Genaev, A. M.; Vasiliev, V. G.; Shubin, V. G. Org. Biomol. Chem. 2012, 10, 2282.
(26) Yan, Y.; Zeitler, E. L.; Gu, J.; Hu, Y.; Bocarsly, A. B. J. Am. Chem. Soc. 2013, 135, 14020.
(27) Coetzee, J. F.; Kolthoff, I. M. J. Am. Chem. Soc. 1957, 79, 6110.
(28) Bausch, M. J.; Gaudalupe-Fasano, C.; Koohang, A. J. Phys. Chem. 1991, 95, 3420. (29) Fukuda, E. K.; McIver, R. T. J. Phys. Chem. 1983, 87, 2993.
ELECTROCHEMICAL HYDROGENATION OF A Ni(II) COMPLEX TO FORM A SURFACE-ADSORBED HYDROGEN-EVOLVING SPECIES
Portions of this work are excerpted with permission from:
The pursuit of sunlight-to-fuels technologies has motivated researchers to explore electrocatalysts for the production of chemical fuels like hydrogen.1–3 These efforts have spanned both homogeneous and heterogeneous systems. Molecular electrocatalysts are particularly attractive targets of study because their electronic structure can be readily tuned through ligand modification,4 their secondary coordination sphere can be modified to promote substrate stabilization or provide a substrate relay,5 and mechanistic and kinetic information can be gleaned through electrochemical6 or spectroscopic methods.1,7 Through these studies, clear correlations have been made between molecular structure and catalytic activity.
While molecular catalysts offer an ideal platform with which to study the hydrogen evolution reaction, their stability under electrocatalytic conditions must be carefully assessed. What begins as a molecular complex may degrade to a new active or inactive molecular or heterogeneous species.8,9 If, during electrocatalysis, a molecular species degrades or otherwise transforms into a heterogeneous species, the resulting product may adsorb to the electrode. Provided that the adsorption is strong, rinsing the electrode and analyzing its electrochemical response in a solution containing only substrate can reveal whether a heterogeneous active species has deposited on the electrode.10,11 Characterization of the electrode surface by various surface techniques can aid in the identification of the heterogeneous active species. These methods have already been successfully employed to identify the transformation of a nickel bis(benzenedithiolate) complex into a Ni-S film active for electrochemical hydrogen evolution.10 Several cobalt complexes have been found to degrade into electrode-adsorbed cobalt nanoparticles also active for hydrogen evolution.12–15 Very recently, decomposition of a nickel bisglyoximato complex to nickel-based nanoparticles was also reported.16 An alternative diagnostic for heterogeneous electrochemical catalysis is the appearance of irreversible prewaves prior to the onset of the electrocatalytic wave in cyclic voltammetry (CV). In several careful recent studies10,13–16 these prewaves have been proposed to represent the modification of the precatalyst by electrons and substrate (e.g., protons), which, in reported cases, initiates degradation of the molecular species into a catalytically active heterogeneous species.
even decomposition of molecular species under electrocatalytic conditions are not well understood. Even more poorly understood are the pathways by which degradation occurs. Improved understanding of catalyst decomposition mechanisms will aid in the rational design of next generation catalysts with enhanced stability. Here we examine the electrochemical decomposition mechanism of the molecular nickel species [Ni(N-N-SCH3)2](BF4)2 (N-N-SCH3 =
2-pyridyl-N-(2’-methylthiophenyl)methyleneimine) to form an electrode adsorbed film catalytic for hydrogen evolution and characterize the active material through surface analysis techniques. Our results highlight structural features that are vulnerable under electrocatalytic conditions.
Results and Discussion
[Ni(N-N-SCH3)2](BF4)2 (1, Figure 2.1) was synthesized analogous to literature
methods.17 The structural motifs of 1 are similar to the reported hydrogen evolution catalyst [Ni(pyS)3]– (pyS = pyridine-2-thiolate) and related complexes.18,19 We initially hypothesized
that the loosely coordinated pendant pyridines may act as temporary proton docking sites, capable of positioning protons near the nickel center and promoting H2 production, as invoked
for the [Ni(pyS)3]– system and for a number of nickel bis(diphosphine) complexes that
Figure 2.2 Cyclic voltammograms of 0.2 mM 1 in 100 mM [Bu4N][PF6] acetonitrile at varying
scan rates of 50, 100, 500, 1000, and 2000 mV/s. Both waves exhibit a linear trend with respect to the square root of the scan rate. The first redox event appears highly reversible, while the second redox event appears quasi-reversible, possibly due to slow ligand reorganization upon oxidation.
Peak currents varied linearly with scan rate (𝑣1/2), as anticipated for a diffusion
controlled process, indicating 1 is a homogeneous species.23 Additionally, a final irreversible reduction is observed (𝐸 = −2.0 V) with twice the intensity and peak integration of the NiII
/NiI reduction. The wave is likely the direct reduction of the [N-N-SCH3] ligands, as suggested by
voltammograms of the ligand alone (Figure 2.3).
positively shifted from the free ligand reduction, but the relative current densities are similar. All voltammograms were recorded at 100 mV/s in 100 mM mM [Bu4N][PF6] acetonitrile.
Addition of CF3COOH (p𝐾aMeCN = 12.6524) yields a new, irreversible reduction with Ep,c
= −0.98 V (Figure 2.4), followed by a second, larger irreversible wave with an onset near −1.10 V, suggesting electrocatalytic proton reduction. Direct reduction of CF3COOH occurs at
more negative potentials.25
Figure 2.4 Top: Voltammograms of 0.39 mM 1 with additions of 0 to 20 eq. (7.8 mM) of CF3COOH at 100 mV/s in a 100 mM [Bu4N][PF6] CH3CN solution. Bottom: The peak current of
the prewave relative to the one-electron reduction of the catalyst in the absence of acid (𝐢𝐩 = peak current, 𝐢𝐩𝟎 = peak current of NiII/NiI reduction in absence of acid).
Figure 2.5. Cyclic voltammograms of a solution of 0.196 mM 1 with 2.6 mM CF3COOH and a
solution of 0.392 mM 2-pyridyl-N-(2’-methylthiophenyl)methyleneimine ([N-N-SCH3])with 5.2
mM CF3COOH. The ligand only solution is twice the concentration of the precatalyst solution,
as the precatalyst has two ligands per nickel. In the absence of acid (Figure 2.3), peak integration found that the stoichiometric ratio of prewave : ligand hydrogenation as 1:2, indicating 1 electron per ligand. In the presence of acid, the two electron ligand reduction transforms into a four electron ligand hydrogenation (2 electrons/ligand). All voltammograms were recorded at 100 mV/s in 100 mM mM [Bu4N][PF6] acetonitrile.
Table 2.1 Peak integrations of the prewave of 1, ligand reduction, and direct ligand hydrogenation relative to the NiII/NiI reduction. As noted in Figure and Figure 2.5, the concentration of ligand for direct ligand reduction and hydrogenation peak integration was twice that of the concentration of 1, as required of the complex being ligated by two ligands.
NiII/NiI Direct Ligand Reduction Direct Ligand Hydrogenation Prewave
# e- passed 1.00 1.92 4.08 2.99*
*The prewave integration is a combination of the two electron ligand hydrogenation and a single electron NiII/NiI reduction.
The observed prewave is very similar to a feature observed for CH3CN solutions of a
cobalt clathrochelate complex and perchloric acid, where a limiting six electron stoichiometry was observed.15 A net six electron, six proton ligand hydrogenation of the three glyoxime ligands was proposed for the cobalt clathrochelate compound.15 Likewise, a net four electron, four proton ligand hydrogenation was similarly suggested for the related cobalt and nickel bisglyoximato compounds.13,16 Similar to these glyoxime ligands, the N-N-SCH3 ligands of 1
contain a C=N bond. We thus postulate that the prewave feature observed corresponds to hydrogenation of this imine functionality.
of 1, the ligands of 2 conform to a facial arrangement. In the absence of acid, a reversible reduction corresponding to the NiII/I redox couple of 2 is observed (𝐸1/2= −1.14 V vs Fc+/Fc), and, in contrast to 1, an irreversible wave, attributed to the NiI/0 couple, is seen (𝐸𝑝,𝑐 = −1.42 V
vs Fc+/Fc) (Figure 2.6). As anticipated, no prewave is observed upon the addition of acid, yet catalytic waves similar to those observed in analogous scans of 1 appear (Figure 2.7). The catalytic waves of 2 pass more current than the respective scans of 1, likely the result of proton depletion near the electrode surface from the ligand hydrogenation of 1. The lack of a prewave for 2, yet an otherwise similar electrochemical response to 1, provides further evidence that the prewave corresponds to an electrochemical hydrogenation of the C=N bonds of 1. UV-vis studies of both 1 and 2 reveal no chemical changes to either complex upon acid titration in the absence of reductant other than reversible protonation of the sp3 hybridized nitrogens in 2.
Figure 2.6 Cyclic voltammograms of 0.20 mM 1 and 2 without acid at 100 mV/s and with 0.1 M [Bu4N][PF6]. The NiII/NiI reduction of 1 is reversible (dotted trace) and the NiI/Ni0 reduction is
Figure 2.7 Acid titrations of 0.5, 4, and 10 eq. of [CF3COOH] into equimolar solutions of 1 and 2 (0.39 mM). The black traces are the respective acid-free voltammograms. Voltammograms recorded at 100 mV/s in 100 mM [Bu4N][PF6] CH3CN solution.
As the prewave feature seen in the CV of 1 indicates a chemical transformation is initiated under electrocatalytic conditions, the catalytic responses of both 1 and 2 were investigated. For 1, the second, large wave increases linearly with acid concentration up to 100 eq. (Figure 2.8), as anticipated for a catalytic response.26
Figure 2.8 Cyclic voltammograms of a solution of 1 (0.096 mM) with acid additions of 6.8, 13.6, 27.3, and 54.5 eq. of CF3COOH. All voltammograms were recorded at 100 mV/s in 100
mM [Bu4N][PF6] acetonitrile solution. Inset: The dashed linear line was fit to the peak
To evaluate the possibility that a catalytically active, surface-adsorbed heterogeneous species is formed during the cathodic sweep of 1 in the presence of acid, a rinse test10,11 was conducted. Using a freshly polished electrode in a solution of 1 and acid (0.20 mM 1, 13.6 eq. CF3COOH), the potential was scanned from –0.70 V to –1.80 V vs. Fc+/Fc. The electrode was
then removed from the solution, rinsed with CH3CN, and scanned over the same range in a fresh
acid-only solution, generating a voltammogram exhibiting a similar catalytic wave to that observed in the first scan, but with the absence of the prewave (Figure 2.9). Of note, no catalytic wave is observed in the acid-only solution if the electrode was not initially scanned beyond the prewave feature (Figure 2.10).
Figure 2.9 In the acidic solution of 1 (0.20 mM 1, 13.6 eq. CF3COOH), produced a
Figure 2.10 A) Cyclic voltammogram of a solution of 1 and acid and catalyst. B) Over varying potential ranges, individual electrodes were treated in solutions of the acid and catalyst. Once treated for 180 seconds, each was rinsed with acetonitrile before being submerged in an acid-only solution of equal concentration. C) At a single potential beyond the prewave (–1.16 V), varying treatment times were applied to different electrodes. Each was then scanned in an acid-only solution. All cyclic voltammograms were recorded at 100 mV/s in 100 mM [Bu4N][PF6]
To evaluate deposition conditions more closely, potential steps of varying magnitude were applied to a series of freshly polished electrodes in an acidic solution of 1 before the ‘treated’ electrodes were thoroughly rinsed with CH3CN and submerged in fresh, acid-only solutions.
Similar to the behavior of electrodes in solutions of 1 and acid, increasing the concentration of acid in the acid-only solution with a treated electrode results in linearly increasing catalytic waves up to similar acid eq., (Figure 2.11), further confirming that an active, surface adsorbed species is formed upon electrolysis. At higher acid concentrations, the peak current begins to level out, likely limited by the turnover rate of the active material (Figure 2.8 and 2.11).
Figure 2.11 An electrode treated for 480 s in an acidic solution of 0.19 mM 1 produced these voltammograms in an acid-only solution with subsequent acid titrations. All voltammograms were produced at 100 mV/s in 100 mM [Bu4N][PF6] acetonitrile solution. Inset: The dashed
linear fit line was produced using the peak intensities of the catalytic wave for acid titrations up to 80 equivalents.
A similar rinse test was performed using a solution of 2, in which an electroactive, surface adsorbed species forms (Figure 2.12). In this case, only scans to potentials beyond the NiI/0 reduction potential (–1.65 V) produce catalytic responses in acid-only solutions. However, the electroactive material formed from 2 also deposits in the absence of acid; polarizing the electrode at –1.65 V in an acid-free solution of 2 is sufficient to generate a catalytic film, suggesting the acid is essential for hydrogenation of 1, but electrodeposition of hydrogenated 1
Figure 2.12 In the acidic solution of 2 (0.39 mM 2, 13.6 eq. CF3COOH), the purple trace was
recorded. A separate electrode was treated for 480 s at –1.2 V in this solution, rinsed, and placed in an acid-only solution of equal concentration, yielding the dashed blue trace. The positive shift reflects the time dependence of the film generation. The black trace is of the untreated electrode background. Voltammograms recorded at 100 mV/s in 100 mM [Bu4N][PF6] acetonitrile
Figure 2.13 Chronoamperograms of both glassy carbon and platinum under a variety of conditions. Single glassy carbon and platinum electrodes were held at potentials beyond the prewave in acid-only solutions (orange and yellow). The yellow line decreases linearly as the bulk concentration of protons in solution was changed. Single glassy carbon and platinum electrodes were held at potentials prior to the prewave in a solution of 0.19 mM (1) and 2.6 mM [CF3COOH] for 480 s (pink and red). The glassy carbon electrode under these conditions
produced a chronoamperogram indistinguishable from that of the acid-only glassy carbon chronoamperogram. The platinum electrode under these conditions produced a decaying plot, corresponding to the depletion of protons to the electrode. Finally, glassy carbon and platinum electrodes were held at potentials beyond the prewave in the same catalyst and acid solution as before for 480 s (blue and green), which leveled out to the same current density.
period, suggesting heterogeneous catalysis formation from homogeneous molecular catalysts.7 The current plateaus as the percent ‘untreated’ surface area diminishes as the electrodeposited film forms.
Observation that an identical limiting current is reached for both electrodes during the chronoamperometry measurement indicates that an active material is deposited onto the electrode surfaces. For glassy carbon, this electrodeposited material is a ‘better’ proton reduction catalyst than the unmodified electrode.8 For the case of platinum, an already efficient proton-reduction catalyst, depositing the active material obscures the more active electrode material.
To determine if the electrocatalytic response observed for heterogeneous material produced by 1 resulted in production of hydrogen, a glassy carbon electrode was treated in an acidic solution of 1 for 480 s (at –1.74 V), rinsed, and dried. This treated electrode was then subjected to a controlled potential electrolysis in a 26.1 mM CF3COOH CH3CN solution (0.25 M
[Bu4N][PF6]). Gas chromatography of the headspace confirmed the production of hydrogen
with a Faradaic efficiency of 97% (Figure B.4).
The composition of the active material was evaluated by scanning electron microscopy (SEM), transition electron microscopy (TEM), and X-ray photoelectron spectroscopy (XPS). Large area samples were prepared by electrolyzing solutions of 1 and 2 in the presence of CF3COOH with 1 x 1 x 0.1 cm glassy carbon plates. For comparison, a bare glassy carbon plate
as well as dropcast samples of 1, 2, and [Bu4N][PF6] on gold plated silicon wafers were also
analyzed by XPS.
Figure 2.14 Images of glassy carbon plates electrolyzed in 0.19 mM 1 and 13.6 eq. CF3COOH
for 480s at –1.75 V. TEM images obtained by scraping the film off a treated glassy carbon plate, suspending the material in EtOH, and drop casting on TEM grids. (A) SEM cross-section profile of the deposited film. (B) A top-down view of the film. (C) TEM micrograph showing nanoparticles (dark areas). (D) High resolution TEM of single nanoparticles.
Figure 2.15 Images of glassy carbon plates electrolyzed in 0.19 mM 2 and 13.6 eq. CF3COOH
TEM analysis of film material scraped off the glassy carbon plates revealed that these films contained nanoparticles (Figures 2.14–2.15). Metal nanoparticle deposition from homogeneous precatalysts has previously been observed for cobalt and nickel compounds.13,15,16 Energy-dispersive X-ray spectroscopy (EDS) of the TEM samples confirmed the presence of nickel, sulfur, and oxygen with atomic ratios of Ni:S of 18.2:1 and 14.2:1 for plates treated with
1 and 2, respectively, and atomic ratios of Ni:O of 6.4:1 and 7.6:1. The excess of nickel relative to sulfur and oxygen suggests that the nanoparticles produced are primarily nickel-based.
The Ni 2p XPS peak structure is complex, especially for nickel in oxidation states other than Ni0. The characteristic doublet is often accompanied by satellite peaks due to different final state effects with varying intensities and spacings from the main doublet peaks.27–30 For dropcast samples of 1 and 2, the XPS spectra reflect the atomic ratios and binding energies consistent with the molecular species; however, XPS analysis of the electrolyzed samples reveal starkly different atomic ratios and binding energies from the molecular species (Table 2.2). The differences of the Ni:S:N atomic ratios observed for dropcast samples of 1 (1:1.48:2.93) vs. electrolyzed 1
(1:0.11:0.05) indicates that a transformation is undergone by the molecular species as the active film is generated. The high resolution Ni 2p spectrum of electrolyzed 1 reveals a narrow diagnostic peak at 852.7 eV, corresponding to the Ni 2p3/2 peak of Ni0,27 and a peak at 856.0 eV,
indicating the presence of a second Ni species (Figure 2.16). While the Ni 2p peak at 856.0 eV possibly represents Ni-O interactions,10 the XPS data do not permit absolute assignment. By contrast, the high resolution Ni 2p spectra of dropcast 1 and 2 do not show any evidence of Ni0. The spectrum of electrolyzed 2 is qualitatively indistinguishable from that of 1, supporting the notion that 1 and 2 decompose into the same Ni-containing products during electrolysis.
Table 2.2 Theoretical vs. experimental XPS elemental analysis. All atomic ratio percentages are normalized to the percentage of Ni 2p in respective samples.
Peak Theoretical 1 Dropcast 1 Electrolyzed 1 Theoretical 2 Dropcast 2 Electrolyzed 2
Ni 2p 1.00 1.00 1.00 1.00 1.00 1.00
N 1s 4.00 2.93 0.05 4.00 5.21 0.18
S 2p 2.00 1.48 0.11 2.00 2.22 0.12
Ni:O ratios lies in sample treatment: XPS sampled the deposited material still attached to the substrate, while TEM-EDS analysis involved scrapping the deposit off the substrate followed by dispersion by ultrasonication prior to deposition onto a TEM grid. This dispersion may have separated an amorphous overcoat layer (suggested from the SEM and TEM images) from encompassed nanoparticles. Additionally, while XPS probed a thin surface layer over a large area, TEM-EDS analyzed a smaller portion in bulk. We hypothesize that XPS largely analyzed the amorphous film which appears to surround the nanoparticles while the deeper penetrating TEM-EDS preferentially sampled the bulk composition of the nanoparticles.
Figure 2.16 High resolution XPS spectra of the Ni 2p region. (A) Dropcast 1 onto gold plated silica wafer. (B) Electrolyzed 1 on a glassy carbon plate from a 0.38 mM 1 and 13.6 eq. CF3COOH solution. (C) Dropcast 2 onto gold plated silica wafer. (D) Electrolyzed 2 on a glassy
carbon plate from a 0.38 mM 2 and 13.6 eq. CF3COOH solution. Electrolyzed solutions
contained 0.1 M [Bu4N][PF6] and were held at –1.66 V vs. Fc+/Fc for 480s.
Figure 2.17 Stripping waves produced by single voltammograms of solutions of 0.19 mM 1, 2, or Ni(ClO4)2 and CF3COOH (13.6 eq.). Voltammograms were recorded at 100 mV/s in 100 mM
[Bu4N][PF6] acetonitrile solution.
(B): the acid only solution was stirred between scans, but the switching potential positive of the nickel stripping wave (–0.65 V vs. Fc+/Fc). When (B) is met, catalytic current decreases and the onset shifts negatively upon successive scans. All voltammograms recorded at 100 mV/s in 100 mM [Bu4N][PF6] acetonitrile solution.
Surface analysis and voltammetry measurements both suggest the presence of more than one nickel species on the electrode surface, including Ni0. To determine if Ni0 was the only catalytically active species in the film, or if another nickel species contributed to the catalytic response currents, electrochemical acid titration experiments were performed with solutions of Ni(ClO4)2 ∙ 6H2O (Figure 2.19). A catalytic wave is observed with an onset potential more
negative than produced from either solution of 1 or 2. The difference observed between the catalytic wave onset potentials of 1, 2 and Ni(ClO4)2 ∙ 6H2O further support the surface analysis
identification of two Ni species in electrolyzed samples of 1 and 2 and indicate that more than one nickel species contributes the catalytic activity of the film.
Figure 2.19 Voltammograms of acid titrations of [CF3COOH] into 0.39 mM, solutions of (1),
that of either 1 or 2. All scans were taken at 100 mV/s in 100 mM [Bu4N][PF6] acetonitrile
As the electrodeposition of Ni0 continues throughout the CV for solutions of Ni(ClO4)2, curve
crossing of the catalytic wave is observed on the reverse scan. More catalytically active material is present on the return trace, so higher hydrogen evolution rates may occur.
Taken together, the electrochemical data and surface analyses help elucidate the pathway by which the active, surface adsorbed species is deposited. The lack of a prewave for 2 strongly supports assignment of the prewave observed for solutions of 1 in the presence of acid as C=N hydrogenation. The limiting two electron stoichiometry of this prewave suggests a net two electron, two proton, C=N hydrogenation of a single ligand of 1. Since reduction and hydrogenation of the free ligand in the presence of acid (Figure 2.3 and 2.5) occurs at potentials much more negative than the prewave, this suggests that ligand hydrogenation in 1 occurs via an intramolecular pathway mediated by electrochemically generated NiI, analogous to the mechanism proposed for ligand hydrogenation in the cobalt clathrochelate complex.15 As noted previously, the NiI/0 redox couple of 1 is quasi-reversible while by contrast the NiI/0 redox couple of 2 is irreversible (Figure 2.6). After two one-electron reductions of 2, 22- decomposes. We hypothesize that after the first metal-mediated ligand C=N hydrogenation of 1, the species generated (1*) is electronically more similar to 2, and upon two sequential reductions, 1*2–
decomposes to form multiple electrode-adsorbed active species as identified by electrochemical and XPS analysis.
Surface analysis by XPS, SEM, and TEM support this decomposition pathway by identifying similarities between the decomposition products of 1 and 2, in which both nickel-containing nanoparticles and an additional Ni species are present.
This work joins only a few other studies describing the transformation of a precatalyst to an H2-evolving film and offers new insight into decomposition pathways of coordination
complexes into heterogeneous species. Unlike prior studies where C=N bond hydrogenation is implicated to be responsible for electrochemical prewaves, this work provides compelling evidence that this assignment is correct via comparison with an all-hydrogenated molecular analogue. The susceptibility of C=N bonds towards hydrogenation suggests such structural components should be avoided in the design of molecular electrocatalysts.
(1) Dempsey, J. L.; Winkler, J. R.; Gray, H. B. In Comprehensive Inorganic Chemistry II; Reedijk, J.; Poeppelmeier, K., Eds.; Elsevier: Oxford, 2013; Vol. 8, pp. 553–565. (2) Thoi, V. S.; Sun, Y.; Long, J. R.; Chang, C. J. Chem. Soc. Rev. 2013, 42, 2388.
(3) McKone, J. R.; Marinescu, S. C.; Brunschwig, B. S.; Winkler, J. R.; Gray, H. B. Chem. Sci. 2014, 5, 865.
(4) Redin, K.; Wilson, A. D.; Newell, R.; DuBois, M. R.; DuBois, D. L. Inorg. Chem. 2007, 46, 1268.
(5) Rakowski DuBois, M.; DuBois, D. L. Chem. Soc. Rev. 2009, 38, 62.
(6) Rountree, E. S.; McCarthy, B. D.; Eisenhart, T. T.; Dempsey, J. L. Inorg. Chem. 2014, 53, 9983.
(7) Wasylenko, D. J.; Rodríguez, C.; Pegis, M. L.; Mayer, J. M. J. Am. Chem. Soc. 2014, 2. (8) Widegren, J. a.; Finke, R. G. J. Mol. Catal. A Chem. 2003, 198, 317.
(9) Artero, V.; Fontecave, M. Coord. Chem. Rev. 2005, 249, 1518.
(10) Fang, M.; Engelhard, M. H.; Zhu, Z.; Helm, M. L.; Roberts, J. a. S. ACS Catal. 2014, 4, 90.
(11) Artero, V.; Fontecave, M. Chem. Soc. Rev. 2013, 42, 2338.
(12) Ghachtouli, S. El; Guillot, R.; Brisset, F.; Aukauloo, A. ChemSusChem 2013, 6, 2226. (13) Anxolabéhère-Mallart, E.; Costentin, C.; Fournier, M.; Robert, M. J. Phys. Chem. C 2014,
(15) Anxolabéhère-Mallart, E.; Costentin, C.; Fournier, M.; Nowak, S.; Robert, M.; Savéant, J.-M. J. Am. Chem. Soc. 2012, 134, 6104.
(16) Cherdo, S.; Ghachtouli, S. El; Sircoglou, M.; Brisset, F.; Orio, M.; Aukauloo, A. Chem. Commun. (Camb). 2014, 50, 13514.
(17) Lindoy, L. F.; Livingstone, S. E. Inorg. Chem. 1968, 7, 1149.
(18) Han, Z.; Shen, L.; Brennessel, W. W.; Holland, P. L.; Eisenberg, R. J. Am. Chem. Soc.
2013, 135, 14659.
(19) Han, Z.; Eisenberg, R. Acc. Chem. Res. 2014.
(20) Curtis, C. J.; Miedaner, A.; Ciancanelli, R.; Ellis, W. W.; Noll, B. C.; Rakowski DuBois, M.; DuBois, D. L. Inorg. Chem. 2003, 42, 216.
(21) Bullock, R. M.; Appel, A. M.; Helm, M. L. Chem. Commun. 2014, 50, 3125.
(22) Chatterjee, S. K.; Roy, S.; Barman, S. K.; Maji, R. C.; Olmstead, M. M.; Patra, A. K. Inorg. Chem. 2012, 51, 7625.
(23) Bard, A. J.; Faulkner, L. R. Electrochemical Methods: Fundamentals and Applications; 2nd ed.; John Wiley & Sons, Inc., 2001.
(24) Izutsu, K. Acid-Base Dissociation Constants in Dipolar Aprotic Solvents; IUPAC Chem.; Blackwell Science: Oxford, U.K., 1990.
(25) McCarthy, B. D.; Martin, D. J.; Rountree, E. S.; Ullman, A. C.; Dempsey, J. L. Inorg. Chem. 2014, 53, 8350.
(26) Savéant, J.-M. Chem. Rev. 2008, 108, 2348.
(27) Grosvenor, A. P.; Biesinger, M. C.; Smart, R. S. C.; McIntyre, N. S. Surf. Sci. 2006, 600, 1771.
(28) Nesbitt, H. W.; Legrand, D.; Bancroft, G. M. Phys. Chem. Miner. 2000, 27, 357.
(29) Ratcliff, E. L.; Meyer, J.; Steirer, K. X.; Garcia, A.; Berry, J. J.; Ginley, D. S.; Olson, D. C.; Kahn, A.; Armstrong, N. R. Chem. Mater. 2011, 23, 4988.
(30) Payne, B. P.; Biesinger, M. C.; McIntyre, N. S. J. Electron Spectros. Relat. Phenomena
In the past few decades, much effort has been made to advance the field of hydrogen evolving electrocatalysts.1–3 In the broadest sense, such electrochemical systems can be classified under one of two categories, homogenous or heterogeneous catalysts. Such distinction, however, does not suit all hydrogen-evolving systems. Some molecular complexes, homogeneous by design, are not stable under electrocatalytic conditions and degrade into surface-adsorbed films.4,5 In place of homogeneous activity by the molecular species, such films often contain nanoparticles or other heterogeneous platforms that evolve hydrogen.6–11
The mechanistic evaluation of such degradation is challenging; only a few examples exist that thoroughly characterize such systems.11,12 Very recently, a collection of such metal complexes known to electrochemically degrade to form electrode-adsorbed heterogeneous materials active for hydrogen evolution was published.12 Among those presented are examples of cobalt and nickel containing species and key structural motifs of their respective ligand frameworks are highlighted. One particularly unique example presented is a set of two nickel complexes, Ni(N-N-SCH3)2(ClO4)2 analogues, with related—but slightly modified—ligands.11
One of the complexes, which contained C=N bonds, underwent partial ligand hydrogenation in the presence of acid before devolving to an active material. The analogue, which contained no C=N bonds, degraded to similar products in the presence of acid. The study purported that the presence of C=N bonds should be avoided in the design of future molecular catalysts to avoid potential decomposition pathways. It did not, however, discuss the importance of the metal identity on the decomposition mechanism.
Examples of iron-containing species degrading to hydrogen-evolving films have not yet been reported. The synthesis and examination of such a species would offer the first example of a homogeneous iron complex degrading to a heterogeneous film or potential nanostructures active towards hydrogen evolution. Herein we report the synthesis and electrochemical characterization of Fe(N-N-SCH3)2(ClO4)2, the iron analogue of the Ni(N-N-SCH3)2(BF4)2